Theories and Methods of First Order Ferroelectric Phase Transitions


 Hortense Waters
 2 years ago
 Views:
Transcription
1 16 Theories and Methods of First Order Ferroelectric Phase Transitions C L Wang Shandong University P R China 1. Introduction Most ferroelectrics in practical applications are of first order phase transition, such as barium titanate, lead zirconium titanate, etc. However, theoretical investigation of first order phase transition is much more complicated than that of second order phase transitions. Therefore in the chapter, theoretical treatments of ferroelectric phase transition of first order are summarized. In the next section, results from thermodynamic theory are discussed. This kind of theory is often called Landau theory, LandauDevonshire theory or Landau Devoshire Ginzburg theory in literatures. Basic concepts and definitions such as characteristic temperatures, thermal hysteresis and field induced phase transition are presented. In the third section, effective field approach for first order phase transition is formulised. Even though this approach is a very simple statistic physics method, it supplies a very helpful approach to understand many physical phenomena of first order phase transitions. In the fourth section, results from Ising model in a transverse field under mean field approximation are discussed. Then the equivalence of the model with effective field approach is demonstrated. Also application of Monte Carlo simulation on Ising model with fourspin couplings is included. In the last part, understanding of physical property of relaxor ferroelectrics from point view of first order phase transition is addressed.. Thermodynamic theory of ferroelectrics In this section, thermodynamic theory of first order ferroelectric phase transition is formalized. Free energy is analyzed at first. Then definition of characteristic temperatures is discussed. Afterwards temperature dependence of polarization and hysteresis loops are shown for static situation. At last dynamic behavior of polarization under external electric field is presented. Formalism of thermodynamic description, or Landau theory for ferroelectrics can be found in many classical books (Blinc & Zeks,1974; Lines & Glass, 1977), or from website like wikipedia (http://en.wikipedia.org/wiki/ferroelectricity). Based on Landau theory, the free energy of a ferroelectric material, in the absence of an electric field and applied stress may be written as a Taylor expansion in terms of the order parameter, polarization (P). If a sixth order expansion is used (i.e. eighth order and higher terms truncated), the free energy is given by:
2 76 Ferroelectrics Δ G = α0 TTPPP α 11 PPP α 1 PPPPPP α 111 ( PPP ) 11 ( ) ( ) ( ) x + y + z + α PPP x y z PPP y z x PPP z x y 1 + α13ppp xyz ( )( x y z ) ( x y z ) ( x y y z z x ) where ΔG stands for the free energy difference of ferroelectric phase and that of paraelectric phase, P x, P y, and P z are the components of the polarization vector in the x, y, and z directions respectively. The coefficients, α i,α ij,α ijk must be consistent with the crystal symmetry. To investigate domain formation and other phenomena in ferroelectrics, these equations are often used in the context of a phase field model. Typically, this involves adding a gradient term, an electrostatic term and an elastic term to the free energy. In all known ferroelectrics, α 0 and α 111 are of positive values. These coefficients may be obtained experimentally or from abinitio simulations. For ferroelectrics with a first order phase transition, α 11 is negative, and α 11 is positive for a second order phase transition. The ferroelectric properties for a cubic to tetragonal phase transition may be obtained by considering the one dimension expression of the free energy which is: Δ G= α0 ( T T0 ) Px + α 11Px + α 111Px () 4 6 The shape of above free energy is schematically shown in Fig. 1 at different temperatures for first order phase transitions. In the following numerical calculations, parameter values are set as α 0 =1, T 0 =1, α 11 =1and α 111 =1 in arbitrary unit for simplicity. (1) Fig. 1. Free energy for a first order ferroelectric phase transition at different temperatures There are four characteristic temperatures in the phase transition process, i.e., CurieWeiss temperature T 0, Curie temperature T c, ferroelectric limit temperature T 1 and limit temperature
3 Theories and Methods of First Order Ferroelectric Phase Transitions 77 of field induced phase transition T. The CurieWeiss temperature can be easily accessed experimentally from the CurieWeiss law of dielectric constant ε at paraelectric phase, i.e., C ε p = TT 0 (3) In above expression, C is the CurieWeiss constant, subscript p of ε stands for paraelectric phase. However the Curie temperature is less accessible experimentally. This temperature measures the balance of the ferroelectric phase and the paraelectric phase. At this temperature, the free energy of ferroelectric phase is the same as that of paraelectric phase. When temperature is between T 0 and T c, ferroelectric phase is stable and paraelectric phase is metastable, this can be easily seen in Fig.1. When the temperature is between T c and T 1, ferroelectric phase is in metastable state while paraelectric phase is stable. When the temperature is higher than T 1, ferroelectric phase disappears. Normally, this temperature is corresponding to the peak temperature of dielectric constant when measured in heating cycle. In other words, peak temperature of dielectric constant measured in heating cycle is the ferroelectric limit temperature T 1, not the Curie temperature T c in a more precise sense. Between temperature T 1 and T, ferroelectric state still can be induced by applying an external electric field. The polarization versus the electric field strength is a double hysteresis loop, which is very similar with that observed in antiferroelectric materials. When the temperature is higher than T, only paraelectric phase can exist. The characteristic temperatures T c, T 1 and T can be easily determined from Eq.() of free energy as following. The Curie temperature T c can be obtained from the following two equations; Δ G= α0( Tc T0) Px + α 11Px + α 111Px = 0 (4) 4 6 Δ G = α 3 5 ( TTP ) +α P +α P = P x 0 c 0 x 11 x 111 x 0 The first equation means that the free energy of ferroelectric phase is same as that of paraelectric phase, and the second equation implies that the free energy of ferroelectric phase is in minimum. From above two equations, we can have the expression of the Curie temperature T c as (5) 3 α TT c = α α (6) At the ferroelectric limit temperature T 1, free energy has an inflexion point at Ps, the spontaneous polarization. As can be seen from Fig. 1, when temperature is below T 1, free energy has are three minima, i.e., at P=±Ps, and P=0. Above temperature T 1, there is only one minimum at P=0. The spontaneous polarization can be obtained from the minimum of the free energy as, Δ G = α ( TTP 0 ) x +α 11Px +α 111Px = 0 P x ( ) 4 Px α0t T0 +α 11Px +α 111Px = 0 (7)
4 78 Ferroelectrics Since P x = 0 corresponds to a free energy maxima in the ferroelectric phase, the spontaneous polarization Ps is obtained from the solution of the equation: which is 4 ( TT ) P P α +α +α = (8) x 111 x 0 1 P = α ± α 4α α ( T T ) x α 111 (9) Hence at temperature T 1, we have In a more explicitly form, ( TT ) α 4α α = 0 (10) α11 TT 1 = 0 + (11) 4 α α Between temperature T 1 and T, there are still inflexion points, which means ferroelectric phase can be induced by an external electric field. When temperature is above T, the inflexion points disappear. By taking the second derivative of the free energy Eq.(), we can have the solution of the inflexion points, G Δ = α 4 0( TT 0) + α 11P + α x 111P = x Px 1 Px = 3α ± 3α 0α α 10α 111 ( ) ( T T ) (1) (13) That is the polarization at the inflexion points. The limit temperature of the induced phase transition T can be determined by or ( ) ( TT ) 3α 0α α = 0 (14) α TT = α α (15) The temperature dependence of the spontaneous can be calculated from Eq.(9) by elimination of solutions yielding a negative square root (for either the first or second order phase transitions) gives: Px 1 = α ± α 4α α α 111 ( T T ) (16) The temperature dependence of the spontaneous polarization from above equation is shown in Fig.. The four characteristic temperatures are denoted by light arrows. The dark arrows
5 Theories and Methods of First Order Ferroelectric Phase Transitions 79 indicate the temperature cycles. Theoretical temperature hysteresis is ΔT=T 1 T 0. Experimentally, the temperature hysteresis could be larger than this value because of the polarization relaxation process. The hysteresis loop (P x versus E x ) may be obtained from the free energy expansion by adding an additional electrostatic term, E x P x, as follows: Δ G= α0 ( T T0 ) Px + α 11Px + α111px EP x x (17) 4 6 Δ G = α 3 5 ( TTP ) +α P +α P E = P x 0 0 x 11 x 111 x x 0 (18) ( ) 3 5 E =α TTP +α P +α P (19) x 0 0 x 11 x 111 x Fig.. Temperature dependence of the spontaneous polarization Plotting E x as a function of P x and reflecting the graph about the 45 degree line gives an 'S' shaped curve when temperature is much lower than the transition temperatures, as can be seen from curves in Fig. 3. The central part of the 'S' corresponds to a free energy local maximum, since the second derivative of the free energy ΔG respect polarization P x is negative. Elimination of this region and connection of the top and bottom portions of the 'S' curve by vertical lines at the discontinuities gives the hysteresis loop. Temperatures are labeled by each curve, label of 0.7T 0 in Fig. 3 is for temperature T=0.7T 0, and 1.T is for T=1.T, T 1 stands for T=(T 1 +T )/. When the temperature is below Curie temperature T c, normal ferroelectric hysteresis loops can be obtained. When the temperature is between T 1 and T, double hysteresis loop or pinched loop could be observed. That means ferroelectric state is induced by the applied electric field. When the temperature is higher than T, the polarization versus electric field becomes a nonlinear relation, see 1.T curve in Fig. 3. It should point out that curves in Fig. 3 are obtained under static electric field. Experimental
6 80 Ferroelectrics measurements usually are performed using time dependent electric field, mostly in sine form. Therefore the hysteresis loops obtained experimentally might be different from the shapes shown in Fig. 3. Fig. 3. Static hysteresis loops at different temperatures Dynamic behavior of ferroelectrics from theoretical simulation could be more helpful for understanding the experimental observing. The dynamic property of ferroelectrics can be studied using LandauKhalantikov equation (Blinc & Zeks, 1974) dp δδg = Γ (0) dt δ P where Γ is the coefficient of thermodynamic restoring force. This equation has been employed to investigate the switching characters of asymmetric ferroelectric films (Wang et al., 1999) and the effects of external stresses on the ferroelectric properties of Pb(Zr,Ti)TiO 3 thin films (Song et al., 003). By inserting free energy (17) into Eq.(0), we have dp 3 5 = Γ α ( ) +α +α dt 0 TTP 0 x 11Px 111Px Ex (1) From above equation, hysteresis loops at different temperature and frequency can be obtained with the electric field is in sine form, Ex = E0 sin( ω t) () The hysteresis loops showing in Fig. 4 are at Curie temperature T c, T 1, (T 1 +T )/, T and 1.T with frequency ω=0.001, E 0 =0.5 and Γ=.0. At Curie temperature T c, a normal ferroelectric hysteresis loop is obtained. At temperature T 1, the hysteresis loop is pinched. Between T 1 and T, double hysteresis loop is obtained as expected, see the blue curve in Fig. 4 for temperature T= (T 1 +T )/. However, at temperature T, double hysteresis loop can be
7 Theories and Methods of First Order Ferroelectric Phase Transitions 81 still observed because of the finite value of relaxation time. Higher than T, no hysteresis can be observed, but a nonlinear PE relation curve. Similar shapes of hysteresis loops have been observed in Pb x Sr 1x TiO 3 ceramics recently(chen et al., 009). Fig. 4. Dynamic hysteresis loops at different temperatures with frequency ω= Dark loop is at Curie temperature T c, red curve is for T 1, blue curve for (T 1 +T )/, green curve for T, and dark line for T=1.T. To get insight understanding of the influence of the frequency on the shape of the hysteresis, more hysteresis loops are presented in Fig. 5. The frequency is set as ω=0.001 for green curves, ω=0.01 for red curves and ω=0.03 for blue curves at Curie temperature T c, T 1, (T 1 +T )/ and at T respectively. At Curie temperature T c, see Fig. 5(a), the coercive field increases with increasing of measure frequency, but the spontaneous polarization is less influenced by the frequency. At temperature T 1, this temperature corresponding to the peak temperature of dielectric constant when measured in heating cycle, pinched hysteresis loop can be observed at low frequency, see the green curve in Fig. 5(b). At higher frequency, the loop behaves like a normal ferroelectric loop, see blue curve in Fig.5(b). When temperature is between T 1 and T, as shown in Fig. 5(c) for temperature at T=(T 1 +T )/, typical double hysteresis loop can be observed at low frequency. When the frequency is higher, it becomes a pinched loop. This trend of loop shape can be kept even when temperature is up to T, see curves in Fig. 5(d). Temperature dependence of polarization at different temperature cycles can be also obtained from Eq.(1) with a constant electric field E=0.01. The results are shown in shown in Fig. 6 with different Γ, the coefficient of thermodynamic restore force. The dark line is for the static polarization, red curves are field heating, blue curves are field cooling. Solid lines are for Γ=100, and dashdotted lines are for Γ=10. The temperature hysteresis from the static theory, as indicated by the two dark dash lines, is smaller than that from Landau Khalanitkov theory. In other words, temperature hysteresis ΔT measured experimentally would be usual larger than that from static Landau theory. Also the temperature hysteresis ΔT depends on Γ, since Γ is related with the relaxation time. A larger Γ represents small
8 8 Ferroelectrics relaxation time, or quick response of polarization with electric field. Hence ferroelectrics with long relaxation time, i.e., small Γ, would expect a very larger temperature hysteresis. Fig. 5. Hysteresis loops with frequency ω=0.001 for green curves, ω=0.01 for red curves and ω=0.03 for blue curves at temperature (a) T c ; (b) T 1 ; (c) (T 1 +T )/, (d) T Fig. 6. Temperature dependence of polarization at different temperature cycles. Dark line is for the static polarization. Red curves are field heating, blue curves are field cooling. Solid lines are for short relaxation time(larger Γ), and dashdot lines are for lone relaxation time (small Γ).
9 Theories and Methods of First Order Ferroelectric Phase Transitions Effective field approach The effective field approach has proved to be a simple statistic physics method but valuable way to describe phase transitions (Gonzalo, 006). The main supposition of this model is that each individual dipole is influenced, not only by the applied electric field, but by every dipole of the system. In its simplest form, which takes into account only dipole interactions, describes fairly well the main features of continuous ferroelectric phase transitions, i.e. second order phase transition. The inclusion of quadrupolar and higher order terms into the effective field expression is necessary for describing the properties of discontinuous or first order phase transitions (Gonzalo et al., 1993; Noheda et al., 1993, 1994). The effective field approach has turned out to be successful explaining the composition dependence of the Curie temperature in mixed ferroelectrics systems (Ali et al., 004; Arago et al., 006). A quantum effective field approach has also been developed for phase transitions at very low temperature (Gonzalo, 1989; Yuan et al., 003; Arago et al., 004) in ferroquantum paraelectric mixed systems. In this section, quantum effective field approach is adopted to reveal the influence of the zero point energy on first order phase transitions (Wang et al., 008). We can see that when the zero point energy of the system is large enough and the ferroelectric phase is suppressed, a phase transitionlike temperature dependence of the polarization can be observed by applying an electric field. The effective field, as described in detail in Gonzalo s book (Gonzalo, 006), can be expressed as E E P P P 3 5 eff = +β +γ +δ + (3) where E is the external electric field, and the following terms correspond to the dipolar, quadrupolar, octupolar, etc., interaction. By keeping the first two terms, i.e. dipolar and quadrupolar interaction, gives account of the first order transition. From statistical considerations, the equation of state is, 3 Eeff μ ( EPP + β +γ ) μ PN = μ tanh = Nμtanh kt B kt B where N is the number of elementary dipoles per unit volume, μ is the electric dipole moment, k B is the Boltzmann constant, and T is the absolute temperature. The Curie temperature is given by βnμ TC = k The explicit form of the equation of state can be rewritten from Eq.(4), kt B P E = tanh βpp γ μ Nμ B 1 3 In order to handle easier this expression, following normalization quantities are introduced, E P T kt γn μ e p t = g B ; ; ; βnμ Nμ TC βnμ β (4) (5)
10 84 Ferroelectrics so Eq. (5) is rewritten as or 3 p tanh epg + + p = t (6) et 1 3 = tanh ppgp (7) and as in absence of external field e = 0, p = p S ps + gp t = (8) tanh 3 S 1 ps Fig.7 shows the plot of the normalized spontaneous polarization p S versus normalized temperature t obtained from Eq. (8) for several values of the parameter g. As it is shown in the discussion of the role of the quadrupolar interaction in the order of the phase transition (see Gonzalo et al., 1993; Noheda et al., 1993; Gonzalo, 006), values of g smaller than 1/3 correspond to a second order, or continuous phase transition, and values larger than 1/3 indicate that the transition is discontinuous, that is, first order. In this case, a spontaneous polarization p θ exists at temperature T θ >T C, and then τ θ >1, being Δt = t θ 1 the corresponding reduced thermal hysteresis, which is the signature of the first order transitions. Fig. 7. Temperature dependence of the spontaneous polarization for different quadrupolar interaction coefficient g. The inset shows the polarization discontinuity p θ (g) and the thermal hysteresis temperature Δt(g) in a first order transition.(wang et al., 008) In order to determine p θ (g), deriving in Eq. (8), t p S pθ = 0
11 Theories and Methods of First Order Ferroelectric Phase Transitions 85 and p θ (g) can be obtained from ( p )( gp ) 1 p ( p gp 3 θ θ θ θ θ) tanh + = 0 (9) Substituting p θ (g) in Eq. (8) again we obtain t θ (g). The inset of Fig.7 shows p θ (g) and Δt(g) respectively. It can be seen that Δt grows almost linearly with g and that p θ approaches to a saturation value that, resolving Eq.(9), turns out to be p θ = when g. When a phase transition takes place at very low temperature it is necessary to consider quantum effect. The energy of the system is no longer the classical thermal energy k B T, but the corresponding energy of the quantum oscillator, 1 E = ω 0 + n being E 0 = ħω 0 / the zero point energy, and <n> the average number of states for a given temperature T. From this quantum energy expression we can obtain a new temperature scale T Q (see Arago et al., 004) defined as, 1 1 Q Q ω0 ω 0 + kt 0 / kt B T ω B e 1 k tanh /kt B ( ω ) and then, the corresponding quantum normalized temperature, t Q T Q /T C. If we introduce a new normalization for the zero point energy so we can rewrite, E ω / Ω 0 0 kt = β BC N μ 0 B (30) Q t and Eq. (7) and (8) become respectively, Ω tanh / ( Ω t ) (31) Q 1 3 = (3) et tanh ppgp t Ω p + gp =, e = Q S S tanh ( Ω / t) tanh ps The temperature dependence of the spontaneous polarization can be found from above equation for a given value of g and different values of the parameter Ω. Fig. 8 plots p S (t) with g = 0.8 to ensure it is a first order transition. The influence of the zeropoint energy is quite obvious: when it is small, the phase transition is still of normal first order one. As the zero point energy increases, both the transition temperatures and the spontaneous polarization decrease. The Curie temperature goes to zero for Ω = 1, but no yet t θ, neither the saturation spontaneous polarization does. From the definition of the normalized zero point energy Ω, we can see then that the Curie temperature goes to zero when the zero point energy is the same as the classical thermal energy k B T C. Imposing again the condition of the zero slope, (33)
12 86 Ferroelectrics ( t/ p S )p θ = 0, we can obtain p θ (Ω), and then t θ (Ω), which must be zero when the ferroelectric behavior will be completely depressed. In this way we work out the zero point energy critical value (Ω cf = for g=0.8) that would not allow any ordered state. Furthermore, from the condition t θ (Ω cf, g) = 0, we will find the relationship between the critical zero point energy Ω cf and the strength of the quadrupolar interaction given by the coefficient g. Fig. 9 plots Ω cf (g) that indicates that Ω cf grows almost linearly with g, specially for larger values of g. This means that ferroelectrics with strong first order phase transition feature needs a relative large critical value of zero point energy to depress the ferroelectricity. Fig. 8. Temperature dependence of the spontaneous polarization at different zero point energy. All curves correspond to a quadrupolar interaction coefficient g=0.8. (Wang et al., 008) Above results prove that a ferroelectric material, with strong quadrupolar interaction, undergoes a first order transition (g>1/3) unless its zero point energy reaches a critical value, Ω cf, because in such case the phase transition is inhibited. However, an induced phase transition must be reached by applying an external electric field. Let be a system with g= 0.8, and Ω=1.6, that is a first order ferroelectric with a zero point energy above the critical value and, hence, no phase transition observed. And let us apply a normalized electric field e that will produce a polarization after Eq. (3). Fig. 10 plots p(t) for different values of the electric field. It can be seen that when it is weak (see curves corresponding to 0.01 and 0.0), the polarization attains quickly a saturation value, similar to what is found in quantum paraelectrics. The curve of e=0.03 (see the dashed line) is split into two parts. The lower part would represent a quantum paraelectric state, but the upper part stands for a kind of ferroelectric state. Therefore there exists a critical value between e=0.0 and 0.03, which is the minimum electric field for inducting a phase transition. For 0.04<e<0.06 the induced polarization curve shows a discontinuous step, but as the electric field increases, 0.07, 0.08 and so on, the polarization changes continuously from a large value at low temperature to a relative small value at high temperature, showing a continuous step. So there is another critical electric field somewhere in between 0.05<e<0.07, separates the discontinuous step
13 Theories and Methods of First Order Ferroelectric Phase Transitions 87 and the continuous step of the induced polarization. In fact, this tricritical point would be around e=0.06. It is also important to remark that the abovementioned features of the field induced phase transitions have been observed in lead magnesium niobate (Kutnjak et al., 006), which is a wellknown ferroelectric relaxor. Fig. 9. Quadrupolar interaction dependence of the critical zero point energy Ω cf that depress ferroelectricity. (Wang et al., 008) Fig. 10. Temperature dependence of the field induced polarization for Ω=1.15 and g=0.8. The parameter is the strength of the electric field. (Wang et al., 008)
14 88 Ferroelectrics For further understanding the field induced phase transitions, Fig. 11 shows the hysteresis loops obtained numerically from Eq. (3) and corresponding to the curves displayed in Fig. 10. Double hysteresis loops can be observed when the temperature is lower than a critical point, around t=0.6, suggesting that ferroelectricity can always be induced at very low temperature. When the temperature is higher than this critical value, there is no hysteresis loop and we can just observe a nonlinear p e behaviour (see for instance the case for t=0.7). However, when the electric field is lower than e 0.05, as indicated by the dashed arrow in Fig. 11, no hysteresis loop can be observed. That is the case corresponding to the curves e =0.01 and 0.0 in Fig. 10. The critical electric field able to induce a phase transition logically increases with the increasing of temperature, so at lower temperature region in Fig. 10, we can always have field induced ferroelectricity when the applied electric field is strong enough. Fig. 11. Hysteresis loops at different temperatures for Ω=1.15 and g=0.8. The dashed arrow indicates the minimum electric field needed to induce a ferroelectric state at t=0. (Wang et al., 008) To understand the influence of the zero point energy on the shape of hysteresis loop, here we take the case of g=0.8 at t=0 as example. The corresponding quantum temperature, after Eq. (31), is and then, Eq. (3) becomes Q tt ( = 0) =Ω e 1 3 =Ωtanh ppgp (34) Fig. 1 plots the hysteresis loops calculated after Eq. (34). When the zero point energy is smaller than the critical value Ω cf (Ω cf =1.136, in this case) a normal hysteresis loop is obtained, where the coercive field decreases as zero point energy increases. For the critical value, a double hysteresis loop with zero coercive field is found. But if we continue
15 Theories and Methods of First Order Ferroelectric Phase Transitions 89 increasing the zero point energy, we arrive to a point where no hysteresis loop is found at all. That suggests that above this other critical value, be Ω cp, there is no way to induce a phase transition, even applying a strong field, and the system remains always in a paraelectric state. Fig. 1. Hysteresis loops at zero temperature for different zero point energy values. The critical value of Ω cf is the minimum zero point energy for the system to have ferroelectricity, while the critical value of Ω cp is the maximum zero point energy for the system to get field induced ferroelectricity. (Wang et al., 008) From the analysis of the hysteresis loops in Fig.1 we can determine the critical electric field needed to induce phase transition imposing the conditions, and deriving in Eq. (34) we get, e e = 0, > 0 p p p c hence we obtain, Ω Ω gp = g p > 1 p ( 1 pc ) 1 3 c 0, 6 0 c c (35) ( 3g 1) + ( 3g 1) 6g( Ω ) pc 6g = (36) Substituting p c (g, Ω) obtained after Eq. (36) into Eq. (34) we can get the coercive field e c (p c ) at zero temperature. Besides, as it is showed in Fig. 1, when the zero point energy attains its critical value Ω cf, the coercive field turns out to be zero, so this is another way to check
16 90 Ferroelectrics the quadrupolar interaction dependence of the critical zero point energy Ω cf (g) as displayed in Fig.9. It must be noted the full accordance between the two calculations. At the second critical value of the zero point energy, Ω cp, the hysteresis loop becomes an inflexion ep curve as it can also be observed in Fig.1, so in this case both Eq. (35) must be equal to zero, and by solving the system of equations, it results, ( g ) g 1 Ω cp =, pcp = (37) 1g 6g The phase diagram at zero temperature is shown in Fig. 13. It displays the role of both the quadrupolar interaction strength and the zero point energy on first order phase transitions. On the top of this diagram we find just paraelectric state (PE), while on the bottom left it appears only second order phase transitions (FE: nd order) that correspond to g < 1/3 and Ω 1. On the bottom right (g > 1/3) there are the first order transitions (FE: 1st order) as the critical values of the zero point energy (Ω cf >1) that depress the ferroelectricity grow monotonously with g. Above the curve Ω cf (g) there are induced electric field phase transitions (first order also). They are limited by another curve Ω cp (g) given by Eq. (37) indicating that no phase transition can be observed when the zero point energy of the system is greater than this value. Fig. 13. Phase diagram of zero point energy critical value Ω c versus quadrupolar interaction coefficient g at zero temperature. The second order phase transition region is denoted as FE:nd order, FE:1st order indicates a normal first order transition, ife is the region of induced ferroelectric phase and on the top, PE corresponds to the paraelectric phase. (Wang et al., 008) From above calculations in the framework of effective field approach, it can be seen that a phase transition can be induced by applying an electric field in a first order quantum paraelectric material. There exist two critical values of the zero point energy, one is Ω cf that depress ferroelectricity, and another is Ω cp above which it is impossible to induce any kind
17 Theories and Methods of First Order Ferroelectric Phase Transitions 91 of phase transition independently of the value of the electric field applied. Phase diagram is presented to display the role of both the quadrupolar interaction strength and the zero point energy on the phase transitions features. 4. Ising model with a fourspin interaction Ising model in a transverse field with a fourspin interaction has been used to study the firstorder phase transition properties in many ferroelectric systems. Under the meanfield approximation, firstorder phase transition in ferroelectric thin films (Wang et al., 1996; Jiang et al., 005) or ferroelectric superlattices (Qu, Zhong & Zhang, 1997; Wang, Wang & Zhong, 00) have been systematically studied. Using the Green s function technique, the firstorder phase transition properties in orderdisorder ferroelectrics (Wang et al., 1989) and ferroelectric thin films (Wesselinowa, 00) have been investigated. Adopting the higherorder approximation to the Fermitype Green s function, the firstorder phase transition properties have been studied in the parameter space with respect to the ratios of the transverse field and the fourspin interaction to the twospin interaction for ferroelectric thin films with the uniform surface and bulk parameters (Teng & Sy,005). These works prove that Ising model with fourspin interaction is a successful model for studying first order phase transition of ferroelectrics. In the following, basic formulism under meanfield approximations and Monte Carlo simulation are presented, and the results are discussed. 4.1 Mean field approximation The Hamiltonian of the transverse field Ising model with a fourspin interchange interaction term is (Wang et al., 1989; Teng & Sy, 005): (38) x ( ) zz ( 4) zzzz ii ij i j ijkl i j kl i ij, ijkl,,, H = ΩS J SS J SSSS where Ω is the transverse field, S x and S z are the x and z components of pseudospin1/ operator, J () and J (4) are the twospin and fourspin exchang interaction, subscript i,j,k,l are site number, summation run over only the nearestneighbor sites. Under the mean field approximation (Blinc & Zeks,1974), solutions of Hamiltonian Eq.(38) is, where x F Ω i Si = tanh Fi kt B y Si = 0 z 4 z 3 JSi + J Si + μe z F i Si = tanh Fi kt B For a homogenous system z 4 z z z Fi = Ω + JS ij j + JijklSSS j k l μe < ij> < ijkl>
18 9 Ferroelectrics S = S = S = S = S z z z z z i j k l J = J J = J F = F j 4 ij, ' ijkl, i jkl Therefore we have, ' 3 z JR + JR + μe F RS = i = tanh F kt B (39) ( ' ) 3 F JR J R E The polarization is related to the zcomponent spin average as, = Ω μ (40) z P = NS μ = NR μ (41) Following normalizations are introduced to handle easier this expression, J' Ω 4kT B F 4μE P g ' =, ω=, t =, τ=, e=, p= = R J J J J J Nμ Eq.(39) and (40) can be rewritten as, i ' pgp + 3 /4+ e τ p = tanh τ t (4) p p 3 e τ= ω + + g + ' 8 In the absence of transverse field, i.e., ω=0 in Eq.(43), and by defining quadrupolar contribution factor g as, 4 g ' J g = = 4 4 J Eq.(4) can be rewritten in the same form in Eq. (6), which is obtained from effective field approach. The equivalence of effective field approach and Ising model with four spin couplings under mean field approximation is completely approved. Therefore the critical value of relative quadrupolar contribution is g c =1/3 under mean field approximation for occurrence of first order phase transition. (43) 4. Monte Carlo simulation A well known and useful method to study phase transitions is by means of the Monte Carlo simulations (Binder, 1984). In particular, phase transitions in Ising systems of relatively low dimensions are sufficient to carry out numerical simulations in the vicinity of the transition temperature, providing a good empirical basis to investigate the asymptotic behavior at the phase transition (Gonzalo & Wang, 008). Here Monte Carlo simulation is applied to the
19 Theories and Methods of First Order Ferroelectric Phase Transitions 93 Ising model with fourspin coupling for studying the phase transition behavior, especially checking the critical value from the fourspin coupling strength, or quadrupolar contribution (Wang et al., 010). Monte Carlo method with metropolis algorithm has been used to simulate 3D Ising cubic lattice. The Hamiltonian is same as in Eq.(38), but without the first term, i.e., without including the tunneling term. In this case, the critical value of the fourspin coupling contribution under mean field approximation is 1 J' J' 1 g = c, ( J '/ J) c 1/6 J = J = 3 = The critical fourspin coupling strength is J /J=1/6 from mean field theory, which is a reference value for the Monte Carlo simulations. Periodic boundary condition has been used in the simulations. The lattice size is denoted as N=L L L, where L is edge length. In the Monte Carlo simulation, edge length L=0, 30, 100 are used. Monte Carlo steps are chosen different for different lattices size to achieve an adequate accurate of the results. Fig. 14. Temperature dependence of spin average (a) and reduced average energy of cubic lattice with edge length L=0 and 30 for different fourspin coupling strength J /J. (Wang et al., 010) Simulation is started with relative small lattice size, with edge length L=0 and 30. The temperature dependence of the spin average and the reduced average energy with different fourspin coupling strength are presented in Fig.14. The reduced average energy is defined as the energy with respective to the ground state energy E 0 in the temperature of zero Kelvin. The curve for lattice size L=0 is marked by solid symbols, and that for L=30 is marked by open symbols. The temperature is in the scale of twosite coupling J. As the fourspin coupling strength increases from J /J =0 to J /J =1, the transition temperature is shifted to higher temperature. The decreasing of the average spin and the increasing of the reduced average energy, with increasing temperature around the transition temperature becomes more rapidly as J /J increases. The general difference between L=0 and that of L=30 is marginal except around the transition temperatures. Even though the fourspin coupling
20 94 Ferroelectrics strength (J /J) is much larger than that of the mean field value 1/6, the first order transition characteristic is not such obvious in these two lattice sizes. The temperature dependence of spin average and the reduced average energy of lattice size 100 is shown in Fig.15 for different fourspin coupling strength J /J. The value of J /J increases from 0.0 to 1.1 with increment of 0.1, corresponding the curves from left to right. The general behavior seems similar with that for L=0 and 30 as shown in Fig.14. However, with increasing of the fourspin coupling strength J /J, as can be seen in the most right side curve of J /J=1.1 in Fig.15(a), the spin average drops down around the transition temperature very quickly, showing a discontinuous feature. Similar discontinuous feature can be also seen in the reduced average energy curves in Fig.15(b). The reduced average energy goes up very sharply around the transition temperature for J /J=1.1, as shown in the most right side curve in Fig.15(b). From Fig.15(b), we also notice that there is an inflexion point around the transition temperatures. The reduced average energy at this point is about 1/3 of the ground state energy when J /J is larger. This condition could supply a criterion for determine the transition temperature in the first order phase transition. Fig. 15. Temperature dependence of spin average (a) and reduced average energy (b) of lattice size L =100 for with different fourspin coupling strength J /J. (Wang et al., 010) To determine the transition temperature, we appeal the calculation of the Binder cumulant. The temperature dependence of the Binder cumulant for J /J= 1.0 with different lattice size are shown in Fig.16. For lattice size of L=10, 0, 5, 30 and 40, the Binder cumulant does cross the point at T c =8.148J. For lattice size L is larger, see L= 50, 70, 100 and 150, the Binder cumulant misses the cross point, and drops down from /3 to a very small value at higher temperatures. That means that the transition temperature can not be obtained from the Binder cumulant when the fourspin coupling strength J /J is larger. It is believed that the Binder cumulants in Fig.16 suggesting the transition is of second order when the lattice size is smaller than L=40, and the transition is of first order when the lattice size is larger than L=40. The lattice size L=40 is around the critical lattice size for fourspin coupling strength J /J =1. This also implies that the transition temperature of first order transition is lattice size dependent.
21 Theories and Methods of First Order Ferroelectric Phase Transitions 95 Fig. 16. Binder cumulants for J /J= 1.0 with different lattice sizes. The circle indicates the cross point of the Binder cumulants for lattice size L<40. (Wang et al/, 010) Spin Average <S> J '=0. 00 J '=0. 10 J '=0. 0 J '=0. 30 J '=0. 40 J'=0.50 J '=0. 60 J'=0.70 J '=0. 75 J '=0. 80 J '=0. 90 J '=1. 00 J '= Te mperature T/Tc <E>/E Tempe rature T/Tc J'=0.00 J'=0.10 J'=0.0 J'=0.30 J'=0.40 J '=0.50 J'=0.60 J '=0.70 J'=0.75 J'=0.80 J'=0.90 J'=1.00 J'=1.10 Fig. 17. Temperature dependence of spin average of lattice sizes L=100 for different J /J around the transition temperature. Temperature is scaled by the transition temperature determined by the criterion <E>/E 0 =1/3. (Wang et al., 010) Fig.17 shows the temperature dependence of spin average and the reduced average energy of lattice size 100 as shown in Fig.15, but with temperature rescaled by the transition temperature T C. The transition temperature T C is determined by the criterion of the averaged energy being one third of the ground state energy, i.e., temperature at <E>/E 0 =1/3 being the transition temperature, as circled in Fig.17(b). Results from Monte Carlo simulations on Ising cubic lattices with four spin couplings suggest that, (1) critical value of fourspin coupling strength for occurrence of first order
22 96 Ferroelectrics phase transition is larger than that of mean field theory; () the critical value is lattice dependence. When lattice size is smaller, the phase transition is still of second order; (3) when the phase transition is of first order, the transition temperature can be determined by the average energy being a third of the ground state energy. However, this criterion has not been justified rigorously. 5. Ferroelectric relaxors Ferroelectric relaxors have been drawn much attention because of their high electromechanical performance and unusual ferroelectric properties. Two review articles (Ye, 1998; Bokov & Ye, 006) have summarized the achievements of recent researches on ferroelectric relaxors, especially for lead magnesium nibate (PMN). Basically, there are two categories of explanations about the fundamental physics of their unusual properties. One is based upon the randomness of their compositions and structures, such as Smolenskii s theory and spherical random bond random field model. Another is presumably based upon the experimental phenomenon, such as macromicrodomain and superparaelectric model. In this section, a general explanation of the properties observed in ferroelectric relaxors is proposed after analysis of the later category models (Wang et al., 009). Field induced phase transition and diffused phase transition are reproduced within the framework of effective field approach. Interpretation is started with the experimental results of field induced phase transition in PMN. The temperature dependence of the polarization under different electric field strengths has been obtained (Ye & Schmid, 1993; Ye, 1998). From this relation we can understand that (1) there is no ferroelectric phase transition in the whole temperature range, since there is no spontaneous polarization as the temperature goes down to zero Kelvin; () ferroelectricity can be induced by an external electric field. These imply that the phase transition in PMN is of first order, but the ferroelectricity is depressed in the whole temperature range. To understand these characteristics of ferroelectric relaxors, we can recall the temperature dependence of the spontaneous polarization in a typical normal first order ferroelectric phase transition is shown in Fig.. This implies that PMN is in a paraelectric state, but not far from the ferroelectric state. Apart from the field induced phase transition, the following features should be also found within this temperature range in a normal first order ferroelectric phase transition: (1) a very long relaxation time, because of the critical slow down as the temperature is near the critical temperature. () superparaelectric behavior. Normally there should be a double hysteresis loop observed in this temperature range. However, the double hysteresis loop could be reduced to a superparaelectric shape because of the long relaxation time of the critical slow down. (3) macromicrodomain crossover. As the temperature is much lower than the critical temperature, single domain or macrodomain is expected since it is in ferroelectric state; as the temperature is much higher than the critical temperature, no domain will be observed as it is in paraelectric state. Around the critical temperature, macromicrodomain crossover is expected, i.e., polar nanoregions are forming in this temperature range. All these features have been observed in the ferroelectric relaxors like PMN. The depression of the ferroelectricity in PMN reminds us of the case of quantum paraelectrics SrTiO 3. Therefore the field induced phase transition in a first order phase transition depressed by quantum fluctuation has been investigated within the framework of effective field approach by inclusive of zero point energy (Wang et al., 008). The
23 Theories and Methods of First Order Ferroelectric Phase Transitions 97 temperature dependence of the induced polarization under different electric field is shown in Fig.10. The polarization p and temperature t are in dimensionless unit, the numbers marked in the Fig.10 are the strength of electric field. The major difference between the temperature dependence of the polarization in PMN (Ye & Schmid, 1993; Ye, 1998) and Fig.10 appears at lower temperature range. The polarization of PMN is still difficult to recover by an external field. This suggests that the zero point energy at lower temperature could be much larger than that in the higher temperature. In other words, the zero point energy might be increased with decreasing of temperature. Another evidence of the existence of larger zero point energy can be found from the diffused phase transition in PMN. For the quantum temperature scale with constant zero point energy, the temperature dependence of the dielectric constant has been obtained from Monte Carlo simulation on a Ising model (Wang et al., 00). As the zero point increases, the transition temperature or the peak temperature of the dielectric constant shifts to a lower temperature. As the zero point energy is larger than the critical value, quantum paraelectric feature is obtained. When the zero point energy increases further, the dielectric constant decreases at low temperature. Therefore if the zero point energy changes with temperature and has a larger value only at lower temperature, the dielectric constant will increase as the temperature increases at lower temperature side, and decreases as the temperature increases at higher temperature side. A round dielectric peak will be formed around the temperature of zero point energy dropping down. From above analysis, a temperature dependent form of zero point energy is proposed in the following form (Wang et al., 009) ω ω= (44) + 0 ( TTX ) 1 e α where the zero point energy ω changes around temperature T x from ω 0 at lower temperature to a relative lower value with crossover rate α. By using the same technique of effective field approach as in Refs.(Wang et al., 008; Yuan et al., 003 Gonzalo, 006), with the quantum temperature scale in Eq.(3) and the zero point energy in Eq.(44), the field induce phase transition and diffused phase transition are obtained and shown in Fig.18. All parameters are in dimensionless scale, e stands for the electric field, and k is for the dielectric constant. From Fig.18 we can see that the basic features of field induce phase transition and diffused phase transition observed in relaxor ferroelectric are reproduced. Fig. 18. (a) Field induced phase transition and (b) diffused phase transition. (Wang et al., 009)
24 98 Ferroelectrics The dimensionless quantum temperature scale used in Fig.18 is shown in Fig.19. The solid line represents the quantum temperature scale, and the dashed line is for the real temperature scale. The phase transition temperature is marked by the arrow. That means that the state evolution of relaxor ferroelectric misses the phase transition temperature as the temperature decreases, and reentry of the paraelectric state. The kind of nonergodic behavior is schematically shown in Fig.19(b) for better understanding. Fig. 19. (a) Quantum temperature scale and (b) nonergodic behavior. (Wang et al., 009) Overall, relaxor ferroelectrics like PMN are in a tricritical state of long range ferroelectric order, thermal fluctuations and quantum fluctuations. This critical state can be described by a quantum temperature scale. Following features can be understood from this issue: diffuse phase transition, field induced phase transition, long relaxation time, as well as superparaelectric state, micromacrodomain crossover and nonergodic behavior. However, a more adequate expression of temperature dependence of zero point energy is still needed for better description of the physical behavior in the relaxor ferroelectrics. 6. Final remarks Theoretical methods and models for studying ferroelectric with first order phase transition are definitely not limited to the contents in this chapter. Hopefully results from these theoretical techniques can provide useful information for understanding experimental observations. Heavycomputer relying methods, such as firstprinciple calculations and molecular dynamic simulations etc, have been applied to investigate the physical properties of ferroelectrics. However, fully understanding of the origin of ferroelectrics might need more efforts from both theoretical and experimental side. 7. References Ali, R.A.; Wang, C.L.; Yuan, M.; Wang, Y. X. & Zhong, W. L. (004). Compositional dependence of the Curie temperature in mixed ferroelectrics: effective field approach. Solid State Commun., 19, Arago, C.; Garcia, J.; Gonzalo, J. A.; Wang, C. L.; Zhong, W. L. & Xue, X. Y. (004). Influence of quantum zero point energy on the ferroelectric behavior of isomorphous systems. Ferroelectrics, 301,
25 Theories and Methods of First Order Ferroelectric Phase Transitions 99 Aragó, C.; Wang, C. L. & Gonzalo, J. A. (006). Deviations from Vegard s law in the Curie temperature of mixed ferroelectric solid solutions. Ferroelectrics, 337, Binder, K. (1984). Applications of Monte Carlo Method in Statistical Physics, nd Edition, SpringerVerlag, ISBN X, Berlin Blinc, R. & Zeks, B. (1974). Soft modes in ferroelectrics and antiferroeletrics, NorthHolland Publishing Company, ISBN , Amsterdam Bokov, A. A. & Ye, Z. G. (006). Recent progress in relaxor ferroelectrics with perovskite structure. Journal of Materials Science, 41, 315 Chen, H. W.; Yang, C.R.; Zhang, J.H.; Pei, Y.F. & Zhao, Z. (009). Microstructure and antiferroelectriclike behavior of Pb x Sr 1 x TiO 3 ceramics. J Alloys and Compounds, 486, Gonzalo, J. A. (1989). Quantum effects and competing interactions in crystals of the mixed rubidium and ammonium dihydrogen phosphate systems. Phys. Rev. B, 39, Gonzalo, J. A.; Ramírez, R.; Lifante, G. & Koralewski, M. (1993). Dielectric discontinuities and multipolar interactions in ferroelectric perovskites, Ferroelectrics Letters Section, 15, 916 Gonzalo, J. A. (006). Effective Field Approach to Phase Transitions and Some Applications to Ferroelectrics, World Scientific Press, ISBN , Singapore Gonzalo, J. A. & Wang, C. L. (008). Monte Carlo approach to Phase Transitions, Asociacion Espanola Ciencia y Cultura, ISBN ,Madrid Jiang, Q. & Tao, Y. M. (005). Critical line between the firstorder and the secondorder phase transition for ferroelectric thin films described by TIM. Phys. Lett. A, 336, 16 Kutnjak, Z.; Petzelt, J. & Blinc, R. (006). The giant electromechanical response in ferroelectric relaxors as a critical phenomenon. Nature, 441, Lines, M. E. & Glass A. M. (1997). Principles and Applications of Ferroelectrics and Related Materials, Clarendon Press, ISBN , Oxford Noheda, B.; Lifante, G. & Gonzalo, J.A. (1993). Specific heat and quadrupole interactions in uniaxial ferroelectrics, Ferroelectrics Letters Section, 15, Noheda, B.; Koralewski, M.; Lifante, G. & Gonzalo J. A. (1994). Dielectric discontinuities and multipolar interactions in ferroelectric perovskites, Ferroelectrics Letters Section, 17, 531 Qu, B. D.; Zhong, W. L. & Zhang, P. L. (1997). Ferroelectric superlattice with firstorder phase transition. Ferroelectrics, 197, 36 Song, T. K.; Kim, J. S.; Kim, M.H.; Lim, W.; Kim, Y. S. & Lee, J. C. (003). Landau Khalatnikov simulations for the effects of external streese on the ferroelectric properties of Pb(Zr,Ti)O 3 thin films. Thin Soild Films, 44, Teng, B. H. & Sy, H. K. (005). Transition regions in the parameter space based on the transverse Ising model with a fourspin interaction. Europhys. Lett., 7, Wang, C. L.; Qin, Z. K. & Lin, D. L. (1989). First order phase transition in orderdisorder ferroelectrics. Phys. Rev. B, 40, Wang, C. L.; Zhang, L.; Zhong, W. L. & Zhang, P.L. (1999). Switching characters of asymmetric ferroelectric films. Physics Letters A, 54,
LandauKhalatnikov Simulations for Ferroelectric Switching in Ferroelectric Random Access Memory Application
Journal of the Korean Physical Society, Vol. 46, No. 1, January 2005, pp. 5 9 LandauKhalatnikov Simulations for Ferroelectric Switching in Ferroelectric Random Access Memory Application Tae Kwon Song
More informationSize dependence of domain patterns in a constrained ferroelectric system
JOURNAL OF APPLIED PHYSICS VOLUME 89, NUMBER 1 15 JUNE 001 Size dependence of domain patterns in a constrained ferroelectric system Rajeev Ahluwalia and Wenwu Cao a) Materials Research Laboratory, The
More informationNONLINEAR BEHAVIOUR OF A RESONANT CIRCUIT WITH FERROELECTRIC CERAMIC CAPACITOR
ANALELE ŞTIINŢIFICE ALE UNIVERSITĂŢII "AL.I.CUZA" DIN IAŞI Tomul XLIXLII, s.i.b.fasc.2 Fizica Solidelor  Fizică Teoretică, 19981999 NONLINEAR BEHAVIOUR OF A RESONANT CIRCUIT WITH FERROELECTRIC CERAMIC
More informationUnder normal circumstances, even polar materials do not display a net dipole moment. As a consequence there are no electric dipole equivalents of bar
CRYSTAL SYMMETRY: Crystal structures can be divided into 32 classes, or point groups, according to the number of rotational axes and reflection planes they exhibit that leave the crystal structure unchanged.
More informationLandau Theory of Second Order Phase Transitions
Landau Theory o Second Order Phase Transitions Order Parameter Second order phase transitions occur when a new state o reduced symmetry develops continuously rom the disordered (high temperature) phase.
More informationFerroelectric Capacitors
Ferroelectric Capacitors Introduction The ability of a substance to retain electric polarization in absence of external field bias, is called ferroelectricity (FE). Although this phenomenon, first reported
More informationPMNPT(40%) 7/9/2014 Physics 403 Summer
PMNPT(40%) 7/9/2014 Physics 403 Summer 2014 1 Ferroelectricity. outline Ferroelectricity. Definition Discovery Main properties Phenomenological theory Some materials Relaxors Applications 7/9/2014 Physics
More informationFerroelectricity. Phase transition. Material properties
Ferroelectricity. Phase transition. Material properties BaTiO 3 DKDP KDP PZNPT(9%) PMNPT(30%) PMNPT(40%) 4/22/2014 Physics 403 Spring 2014 1 Ferroelectricity. outline Ferroelectricity. Definition Discovery
More informationNOVACAP TECHNICAL BROCHURE G. DIELECTRIC PROPERTIES
G. DIELECTRIC PROPERTIES There are additional electrical properties characteristic of dielectrics which greatly determine the merit of performance of these materials in capacitor applications. INSULATION
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationUniversality and the fivedimensional Ising model
EUROPHYSICS LETTERS 10 June 1997 Europhys. Lett., 38 (8), pp. 565570 (1997) Universality and the fivedimensional Ising model H. W. J. Blöte and E. Luijten Department of Physics, Delft University of Technology
More informationThe Monte Carlo Method in Quantum Mechanics. Colin Morningstar Carnegie Mellon University
The Monte Carlo Method in Quantum Mechanics Colin Morningstar Carnegie Mellon University Overview will present a detailed description of a Monte Carlo calculation of a simple quantum mechanical system
More informationY. L. Wang, A. K. Tagantsev, D. Damjanovic, and N. Setter arxiv:condmat/ v1 [condmat.mtrlsci] 27 Mar 2006
Anharmonicity of BaTiO 3 single crystals Y. L. Wang, A. K. Tagantsev, D. Damjanovic, and N. Setter arxiv:condmat/0603688v1 [condmat.mtrlsci] 27 Mar 2006 Ceramics Laboratory, EPFLSwiss Federal Institute
More informationCapacitance and Ferroelectrics
Ram Seshadri MRL 2031, x6129 seshadri@mrl.ucsb.edu; http://www.mrl.ucsb.edu/ seshadri/teach.html Capacitance and Ferroelectrics A voltage V applied across a capacitor of caacitance C allows a quantity
More informationSupplemental material for: Twodimensional melting under quenched disorder
Supplemental material for: Twodimensional melting under quenched disorder July 30, 2013 1 Timeaveraged orientational order Fig. 4 of the main article shows the analysis for the experimental data. Figure
More informationValence Electron Charge Density Application to EAM Potential Theory P. Mitev (1), E. Vamvakopoulos (1), G.A. Evangelakis (1), Efthimios Kaxiras (2)*
Valence Electron Charge Density Application to EAM Potential Theory P. Mitev 1), E. Vamvakopoulos 1), G.A. Evangelakis 1), Efthimios Kaxiras 2)* 1) Department of Physics, University of Ioannina, Ioannina,
More informationFrequency And Temperature Dependence Of The Dielectric Constant In Ba 1x Sr x TiO 3 Pellets
Frequency And Temperature Dependence Of The Dielectric Constant In Ba x Sr x TiO 3 Pellets S. Vaitsi, E. Hristoforou Laboratory of Physical Metallurgy, School of Mining and Metallurgy Engineering National
More informationFiniteSize Lattice Effects in Potts Model
FiniteSize Lattice Effects in Potts Model Sasha Soane and Conner Galloway MIT Department of Physics (Dated: May 15, 2008) We explore finitesize effects in the context of a 2dimensional Potts model on
More informationPIEZO CERAMICS. Noliac Group develops and manufactures piezoelectric. zirconate titanate (PZT) of high quality and tailored for custom
Noliac Group develops and manufactures piezoelectric zirconate titanate (PZT) of high quality and tailored for custom Piezoelectric components may be used as e.g.: Actuators Sensors Generators Transducers
More informationBranislav K. Nikolić
Monte Carlo Simulations in Statistical Physics: Magnetic PhaseTransitions in the Ising Model Branislav K. Nikolić Department of Physics and Astronomy, University of Delaware, U.S.A. PHYS 460/660: Computational
More informationInteraction effects in magnetic oxide nanoparticle systems
PRAMANA c Indian Academy of Sciences Vol. 65, No. 4 journal of October 2005 physics pp. 739 743 Interaction effects in magnetic oxide nanoparticle systems RAKSHA SHARMA 1, C PRATIMA 2, SUBHALAKSHMI LAMBA
More informationarxiv:condmat/ v1 13 Jul 1993
POLFISTH.06/93 arxiv:condmat/9307023v1 13 Jul 1993 MEAN FIELD RENORMALIZATION GROUP FOR THE BOUNDARY MAGNETIZATION OF STRIP CLUSTERS Alessandro Pelizzola a and Attilio Stella b a Dipartimento di Fisica,
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationEM4: Magnetic Hysteresis
CHALMERS UNIVERSITY OF TECHNOLOGY GÖTEBORG UNIVERSITY EM4: Magnetic Hysteresis Lab manual (version 1.001a) Students:... &... Date:... /... /... Laboration passed:... Supervisor:... Date:... /... /... Raluca
More informationClassical and quantum anisotropic Heisenberg antiferromagnets
Classical and quantum anisotropic Heisenberg antiferromagnets W. Selke 1, G. Bannasch 1,2, M. Holtschneider 1, R. Leidl 1, I.P.McCulloch 3, D. Peters 1, and S. Wessel 4,1 (1) Institut für Theoretische
More informationMonte Carlo Simulation
Chapter 4 Monte Carlo Simulation Due to the complexity of the problem, treating irregular spin systems with competing interactions in thermal equilibrium and nonequilibrium, we are forced to use Monte
More informationReal Analysis: Differential Calculus
Real Analysis: Differential Calculus 1 1. OneVariable Calculus: Differentiability of Functions Slope of a Linear Function: The slope of a linear function f measures how much f(x) changes for each unit
More informationEXIT TIME PROBLEMS AND ESCAPE FROM A POTENTIAL WELL
EXIT TIME PROBLEMS AND ESCAPE FROM A POTENTIAL WELL Exit Time problems and Escape from a Potential Well Escape From a Potential Well There are many systems in physics, chemistry and biology that exist
More informationAnomalous Synchrotron Xray Scattering Studies of Nanodomains in Pb(Mg 1/3 Nb 2/3 )O 3
Anomalous Synchrotron Xray Scattering Studies of Nanodomains in Pb(Mg 1/3 Nb 2/3 )O 3 A. Tkachuk, Haydn Chen, P. Zschack and E. Colla Department of Materials Science and Engineering and Frederick Seitz
More informationOptimization of energy storage density in ceramic capacitors
J. Phys. D: Appl. Phys. 29 (1996) 253 258. Printed in the UK Optimization of energy storage density in ceramic capacitors N H Fletcher, A D Hilton and B W Ricketts Division of Applied physics, CSIRO, Bradfield
More informationElectroceramics Prof. Ashish Garg Department of Materials Science and Engineering Indian Institute of Technology, Kanpur.
Electroceramics Prof. Ashish Garg Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Lecture  30 Again, we start a new lecture. We will just go through the last lecture
More informationPTC Thermistors [From Philips Data Handbook PA ]
PTC Thermistors [From Philips Data Handbook PA02 1989] 1. GENERAL Positive Temperature Coefficient (PTC) thermistors exhibit a high positive temperature coefficient of resistance. They differ from Negative
More informationChapter 18. Thermal Properties of Matter. Dr. Armen Kocharian
Chapter 18 Thermal Properties of Matter Dr. Armen Kocharian Molecular Model of an Ideal Gas The model shows that the pressure that a gas exerts on the walls of its container is a consequence of the collisions
More informationSimulations: The Ising Model
Simulations: The Ising Model Asher Preska Steinberg, Michael Kosowsky, and Seth Fraden Physics Department, Brandeis University, Waltham, MA 02453 (Advanced Physics Lab) (Dated: May 5, 2013) The goal of
More information8 Flat Plate Analysis
8 Flat Plate Analysis 8.1 Introduction A flat plate is generally considered to be a thin flat component that is subjected to load conditions that cause deflections transverse of the plate. Therefore, the
More informationMaterials and Devices in Electrical Engineering
Examination Materials and Devices in Electrical Engineering Monday 19 th of March, 14:00 to 16:00, room 108 FZU/AVG It is allowed to use any kind of media (books, scripts, overheads, notes,...) during
More informationChapter 5. The Second Law of Thermodynamics
Chapter 5 The Second Law of Thermodynamics Learning Outcomes Demonstrate understanding of key concepts related to the second law of thermodynamics, including alternative statements of the second law, the
More informationRelationship between galvanomagnetic phenomena and bulk elasticity in magnetcontaining
Transworld Research Network 37/661 (2), Fort P.O., Trivandrum695 023, Kerala, India Magnetism and Laws of Bulk Elasticity, 2009: 17 ISBN: 9788178953793 Editors: P.I. Polyakov and T.A. Ryumshyna 1
More informationRecent development in piezoelectric materials used for actuators and sensors applications
Recent development in piezoelectric materials used for actuators and sensors applications Dragan Damjanovic, Ceramics Laboratory, Materials Institute Swiss Federal Institute of Technology  EPFL Lausanne
More informationFerromagnetic Properties of BondDilution and Random Positive or Negative Uniaxial Anisotropy Blume Capel Model
Commun. Theor. Phys. (Beijing, China) 42 (2004) pp. 789 794 c International Academic Publishers Vol. 42, No. 5, November 15, 2004 Ferromagnetic Properties of BondDilution and Random Positive or Negative
More informationPearson Algebra 2 Common Core 2015
A Correlation of Algebra 2 Common Core to the Common Core State Standards for Mathematics High School , Introduction This document demonstrates how meets the Mathematics High School, PARRC Model Content
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationMonte Carlo Simulation technique. S. B. Santra Department of Physics Indian Institute of Technology Guwahati
Monte Carlo Simulation technique S. B. Santra Department of Physics Indian Institute of Technology Guwahati What is Monte Carlo (MC)? Introduction Monte Carlo method is a common name for a wide variety
More informationElasticity and Equations of State
Elasticity and Equations of State The way planets deform depends primarily upon the elastic properties of the constituent polycrystalline materials. In particular, the speed of body waves passing through
More informationHomologous onset of double layer convection
PHYSICAL REVIEW E 8, 46316 29 Homologous onset of double layer convection F. H. Busse* and M. Petry Physikalisches Institut, Universität Bayreuth, D9544 Bayreuth, Germany Received 5 February 29; published
More informationI. Thermodynamics. I.A Fundamental definitions. Thermodynamics is a phenomenological description of equilibrium properties of macroscopic
I. Thermodynamics I.A Fundamental definitions Thermodynamics is a phenomenological description of equilibrium properties of macroscopic systems. As a phenomenological description, it is based on a number
More informationDetermination of Molecular Weight by Freezing Point Depression
Determination of Molecular Weight by Freezing Point Depression Freezing point depression is a kind of colligative properties as treated in high school chemistry course. Normally used alcohol or mercury
More informationPart 2: polarization a microscopic view
Dielectrics Part 2: polarization a microscopic view Ryszard J. Barczyński, 2010 Politechnika Gdańska, Wydział FTiMS, Katedra Fizyki Ciała Stałego Materiały dydaktyczne do użytku wewnętrznego The mechanisms
More informationChapter 12 Electrical Properties
Chapter 12 Electrical Properties Concept Check 12.1 Question: If a metallic material is cooled through its melting temperature at an extremely rapid rate, it will form a noncrystalline solid (i.e., a metallic
More informationOhio State Common Core Standards for Mathematics K 12 TECHNOLOGY FOCUS
Ohio State Common Core Standards for Mathematics K 12 TECHNOLOGY FOCUS INTRODUCTORY PRINCIPLES Use appropriate tools strategically. Mathematically proficient students consider the available tools when
More information4. Thermodynamics of Polymer Blends
4. Thermodynamics of Polymer Blends Polymeric materials find growing applications in various fields of everyday life because they offer a wide range of application relevant properties. Blending of polymers
More informationThermal conductivity of metals
Thermal conductivity of metals 1. Overview of heat transfer phenomena Heat transfer is the transition of thermal energy from a heated item to a cooler item. When an object or fluid is at a different temperature
More informationSolutions to Laplace s Equations III
Solutions to Laplace s Equations III Lecture 15: Electromagnetic Theory Professor D. K. Ghosh, Physics Department, I.I.T., Bombay Laplace s Equation in Spherical Coordinates : We continue with our discussion
More informationPhysics 53. Thermal Physics 2. I have concluded that all of man's troubles have one cause, that he cannot sit still in a room by himself.
Physics 53 Thermal Physics 2 I have concluded that all of man's troubles have one cause, that he cannot sit still in a room by himself. Pascal Average energy of a molecule Toward the end of the 19th century
More informationElectrical and optical properties of materials
Electrical and optical properties of materials JJL Morton Electrical and optical properties of materials John JL Morton Part 3: Piezo pryo and ferroelectricity We have already seen in the discussion
More informationAnalysis of Numerical Errors in the DSMC Method
Analysis of Numerical Errors in the DSMC Method D. A. Fedosov, S. V. Rogasinsky, M. I. Zeifman, M. S. Ivanov, A. A. Alexeenko and D. A. Levin Department of Aerospace Engineering, Pennsylvania State University,
More informationGlobal Seasonal Phase Lag between Solar Heating and Surface Temperature
Global Seasonal Phase Lag between Solar Heating and Surface Temperature Summer REU Program Professor Tom Witten By Abstract There is a seasonal phase lag between solar heating from the sun and the surface
More informationarxiv:condmat/ v1 [condmat.soft] 22 May 1997
SI9708 arxiv:condmat/9705222v1 [condmat.soft] 22 May 1997 Universal Shorttime Behaviour of the Dynamic Fully Frustrated XY Model H.J. Luo, L. Schülke and B. Zheng Universität GH Siegen, D 57068 Siegen,
More informationAlgebra I End of Course Exam Answer Key Segment I Scientific Calculator Only
Algebra I End of Course Exam Answer Key Segment I Scientific Calculator Only Question 1 Reporting Category: Algebraic Concepts & Procedures Common Core Standard: AAPR.3: Identify zeros of polynomials
More informationChapter 4: Theory of Ferroelectric Capacitance Joe T. Evans, Jr.
Radiant Technologies, Inc. 2835D Pan American Freeway NE Albuquerque, NM 87107 Tel: 5058428007 Fax: 5058420366 www.ferrodevices.com email: radiant@ferrodevices.com Chapter 4: Theory of Ferroelectric Capacitance
More informationPart 1: Principles of Statistical Mechanics and the Boltzmann Distribution
PHYS393 Statistical Physics Part 1: Principles of Statistical Mechanics and the Boltzmann Distribution Introduction The course is comprised of six parts: 1. Principles of statistical mechanics, and the
More informationHandout 12. Ising Model
ME346A Introduction to Statistical Mechanics Wei Cai Stanford University Win 2011 Handout 12. Ising Model February 25, 2011 Contents 1 Definition of Ising model 2 2 Solving the 1D Ising model 4 2.1 Noninteracting
More informationUsing Derivatives. Chapter Using derivatives to identify extreme values. Motivating Questions. Introduction
Chapter 3 Using Derivatives 3.1 Using derivatives to identify extreme values Motivating Questions In this section, we strive to understand the ideas generated by the following important questions: What
More informationHandout 11. Applications to Fluids
ME346A Introduction to Statistical Mechanics Wei Cai Stanford University Win 2011 Handout 11. Applications to Fluids February 23, 2011 Contents 1 Ideal gas model review 1 2 Van der Waals model 2 3 Virial
More informationSize and shape dependent melting temperature of metallic nanoparticles
Materials Chemistry and Physics 88 (2004) 280 284 Size and shape dependent melting temperature of metallic nanoparticles W.H. Qi, M.P. Wang School of Materials Science and Engineering, Central South University,
More informationI. Introduction. A. Ferromagnetic Shape Memory Effect
Abstract The phasefield method has been successfully employed during the past ten years to simulate a wide variety of microstructural evolution in materials. Phasefield models describe the microstructure
More informationLecture 3: Electron statistics in a solid
Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................
More informationarxiv:condmat/ v1 [condmat.mtrlsci] 3 Nov 1998
arxiv:condmat/9811039v1 [condmat.mtrlsci] 3 Nov 1998 SLOW FORCING IN THE PROJECTIVE DYNAMICS METHOD M. A. Novotny a M. Kolesik b and P. A. Rikvold a,c a Supercomputer Computations Research Institute
More informationarxiv:condmat/ v1 19 Dec 1995
Errors in Monte Carlo simulations using shift register random number generators F. Schmid and N.B. Wilding Institute für Physik, Johannes Gutenberg Universität Mainz, D55099 Mainz, Germany. arxiv:condmat/9512135v1
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationIII.10. DETERMINATION OF THE CURIE TEMPERATURE FOR FERRIMAGNETIC MATERIALS
III.10. DETERMINATION OF THE CURIE TEMPERATURE FOR FERRIMAGNETIC MATERIALS 1. Work purpose The determination of the Curie temperature for ferrites. 2. Theory The magnetism of the substances is due to the
More informationToday's lecture: various other methods for computing free energies, including absolute free energies, beyond histogram techniques
Other free energy techniques ChE210D Today's lecture: various other methods for computing free energies, including absolute free energies, beyond histogram techniques Perturbation approaches to free energies
More informationNumerical curve fitting of general order kinetics glow peaks
J. Phys. D: Appl. Phys., 1971, Vol. 4. Printed in Great Britain Numerical curve fitting of general order kinetics glow peaks D. SHENKER and R. CHEN Department of Physics and Astronomy, TelAviv University,
More informationEffects of node buffer and capacity on network traffic
Chin. Phys. B Vol. 21, No. 9 (212) 9892 Effects of node buffer and capacity on network traffic Ling Xiang( 凌 翔 ) a), Hu MaoBin( 胡 茂 彬 ) b), and Ding JianXun( 丁 建 勋 ) a) a) School of Transportation Engineering,
More information3 Numerical Methods for Convection
3 Numerical Methods for Convection The topic of computational fluid dynamics (CFD) could easily occupy an entire semester indeed, we have such courses in our catalog. The objective here is to eamine some
More informationThin Film Bibased Perovskites for High Energy Density Capacitor Applications
..SKELETON.. Thin Film Bibased Perovskites for High Energy Density Capacitor Applications Colin Shear Advisor: Dr. Brady Gibbons 2010 Table of Contents Chapter 1 Introduction... 1 1.1 Motivation and Objective...
More informationarxiv:condmat/ v1 19 Sep 1995
Largescale Simulation of the Twodimensional Kinetic Ising Model arxiv:condmat/9509115v1 19 Sep 1995 Andreas Linke, Dieter W. Heermann Institut für theoretische Physik Universität Heidelberg Philosophenweg
More informationChapter 3: Theory of Paraelectric Capacitance Joe T. Evans, Jr.
Radiant Technologies, Inc. 2835D Pan American Freeway NE Albuquerque, NM 87107 Tel: 5058428007 Fax: 5058420366 www.ferrodevices.com email: radiant@ferrodevices.com Chapter 3: Theory of Paraelectric
More informationFirstOrder System Example #1
FirstOrder System Example # A. Overview Two different firstorder systems will be presented in this example. The first system, G (s) will have its one openloop pole located at the origin of the splane,
More informationQNET Experiment #06: HVAC Proportional Integral (PI) Temperature Control Heating, Ventilation, and Air Conditioning Trainer (HVACT)
Quanser NIELVIS Trainer (QNET) Series: QNET Experiment #06: HVAC Proportional Integral (PI) Temperature Control Heating, Ventilation, and Air Conditioning Trainer (HVACT) Student Manual Table of Contents
More informationarxiv: v1 [condmat.statmech] 16 Dec 2008
Parallelization of Markov chain generation and its application to the multicanonical method arxiv:0812.2964v1 [condmat.statmech] 16 Dec 2008 Takanori Sugihara a, Junichi Higo b, and Haruki Nakamura c
More informationA Conceptual Introduction to the Physics of Magnetic Particles. Tim St Pierre School of Physics The University of Western Australia
A Conceptual Introduction to the Physics of Magnetic Particles Tim St Pierre School of Physics The University of Western Australia Outline of Lectures Lecture 1 Magnetic Moments and Magnetic Fields Magnetic
More informationThermodynamic Branch in the Chemical System Response to External Impact
1 Thermodynamic Branch in the Chemical System Response to External Impact INTRODUCTION. B. Zilbergleyt I. Complex behavior of chemical systems is one of the more attractive and, at the same time, one of
More informationEffect of coupling strength on magnetic properties of exchange spring magnets
OURNAL OF APPLIED PHYSICS VOLUME 94, NUMBER 10 15 NOVEMBER 2003 Effect of coupling strength on magnetic properties of exchange spring magnets Vamsi M. Chakka, Z. S. Shan a), and. P. Liu b) Department of
More informationDynamics of Rigid Bodies. (Most of the material presented in this chapter is taken from Thornton and Marion, Chap. 11.)
Chapter 9. Dynamics of Rigid Bodies Most of the material presented in this chapter is taken from Thornton and Marion Chap. 11. 9.1 Notes on Notation In this chapter unless otherwise stated the following
More informationMolecular Dynamics Simulations
Molecular Dynamics Simulations Yaoquan Tu Division of Theoretical Chemistry and Biology, Royal Institute of Technology (KTH) 201106 1 Outline I. Introduction II. Molecular Mechanics Force Field III. Molecular
More informationChapter 3. Mathematical Model of Electromagnetic Brakes
Chapter 3. Mathematical Model of Electromagnetic Brakes 3.1. Introduction Precise mathematical models of the brakes are important for the purpose of simulation and control. In this chapter we review different
More informationCorrelations in mesoscopic magnetic systems F. Gulminelli 1) and Ph. Chomaz 2)
Correlations in mesoscopic magnetic systems F. Gulminelli 1) and Ph. Chomaz 2) LPC Caen, F14050 CAEN Cédex FRANCE GANIL, BP5027, F14076 CAEN Cédex5 FRANCE Subject : The purpose of this proposal is to
More informationLab 4 MODULE γ2 ORDERDISORDER TRANSITIONS. XRay Diffraction Study of Ordering in CoPt System
3.014 Materials Laboratory Dec. 8 th Dec..13 th, 2006 Lab 4 MODULE γ2 ORDERDISORDER TRANSITIONS XRay Diffraction Study of Ordering in CoPt System OBJECTIVES Understand OrderDisorder Transition. Factors
More information7. DYNAMIC LIGHT SCATTERING 7.1 First order temporal autocorrelation function.
7. DYNAMIC LIGHT SCATTERING 7. First order temporal autocorrelation function. Dynamic light scattering (DLS) studies the properties of inhomogeneous and dynamic media. A generic situation is illustrated
More information3.3 Magnetic anomalies
3.3 Magnetic anomalies The characteristics of magnetic anomalies Anomalies of simple shapes The sphere Demagnetization The half space The thin layer The quarter space The magnetic pole A line of poles
More informationSusceptibility and MagnetisationMeasurements
Susceptibility and MagnetisationMeasurements Evan Sheridan with Niall Robertson 11367741 February 2013 Abstract Using a Hall Probe, electromagnet and a set of weighing scales the magnetic phenomena of
More informationIntroduction to Nuclear Lattice Methods
Introduction to Nuclear Lattice Methods Lecture 2: Lattice Theory and Formalism, Scattering on Lattice Dean Lee (NC State) Nuclear Lattice EFT Collaboration Present Status of the Nuclear Interaction Theory
More informationThe laws of thermodynamics
1 The laws of thermodynamics 1.1 The thermodynamic system and processes A physical system containing a large number of atoms or molecules is called the thermodynamic system if macroscopic properties, such
More informationProcessing of Key Pyroelectric Materials
Chapter 3 Processing of Key Pyroelectric Materials 3.1 Introduction Pyroelectric materials have been fabricated in bulk single crystals, ceramic (polycrystalline), films, and composite forms. This chapter
More informationIs there an AlmeidaThouless line in Spin Glasses?
p.1 Is there an AlmeidaThouless line in Spin Glasses? Peter Young email:peter@physics.ucsc.edu Work supported by the Collaborator: H. G. Katzgraber Talk at the APS March Meeting, New Orleans, March 11,
More informationPhysics 112 Magnetic Phase Transitions, and Free Energies in a Magnetic Field
Physics 112 Magnetic Phase Transitions, and Free Energies in a Magnetic Field Peter Young (Dated: March 5, 2012) I. INTRODUCTION There is considerable interest in the effects of magnetic fields on the
More informationOn the Effect of Prestress on the Bistable Behavior of Tapesprings
Keynote ecture Cristina Gentilini, Keith A. Seffen, Simon D. Guest and ucio Nobile/ Proceedings, AES TEA 28 Second International Conference, Cesena, Italy, September 15, 28, pp. 181185 ISBN 978479 Second
More informationGUIDE TO CALCULUS. We have seen in Chapter 18 how a range of business situations and. Objectives
05747_CH26_025056.qxd 7/9/08 10:33 AM Page 25 26 GUIDE TO CALCULUS We have seen in Chapter 18 how a range of business situations and economic relationships can be described mathematically. Using equations,
More informationQuantum Monte Carlo Study of Highpressure solid hydrogen
Quantum Monte Carlo Study of Highpressure solid hydrogen Sam Azadi and Matthew Foulkes Blackett Laboratory Imperial College London Quantum Monte Carlo in the Apuan Alps VIII July2013 Motivation for studying
More information